The formation of gradients of chemical composition, phase distribution or microstructure represents a now fervently pursued concept in the design of advanced engineering components. In light of this concept, a significant progress has been made in the area of functionally graded materials (FGMs). FGMs are of practical interest because a wide gradation of physical and/or chemical properties can be achieved across a given material depending on the material design(Suresh & Mortensen, 1998, Miyamoto et al., 1999, Uemura et al., 2010). Thus, FGM holds continuous changes of the microstructure, the composition and the properties in some specific directions,
There are two types of graded structures of the FGMs, namely continuous structure shown in Fig. 1 (a), and stepwise structure shown in Fig. 1 (b). In the first type, the change in composition and/or microstructure occurs continuously with position. On the other hand in the second type, the microstructure feature changes in a stepwise manner, giving rise to a multilayered structure with interfaces existing between discrete layers (Miyamoto et al., 1999). As will be described in more detail below, the continuous graded structure can be created by a centrifugal force.
In the past, many kinds of processing methods for FGM have been proposed(Suresh & Mortensen, 1998, Miyamoto et al., 1999, Uemura et al., 2010). Powder metallurgy is one of the most important methods of producing FGMs. An example of a typical fabrication process by the powder metallurgy is schematically illustrated in Fig. 2. At first, material A and material B are weighed and mixed, as shown in Fig. 2 (a). The each mixed-powder is mixed uniformlyby a V-shape mill, as shown in Fig. 2 (b). Next step is stepwise staking of premixed powder according to a predesigned spatial distribution of the composition (Fig. 2 (c)). Last step is a sintering. Spark plasma sintering (SPS),shown in Fig. 2 (d),is one of the more advanced sintering methods,and it makes possible sintering high quality materials in short periods by charging the intervals between powder particles with electrical energy and high sintering pressure. However, usually the FGM fabricated by this method should have the stepwise structure,and it is difficult to produce the FGMs with continuous gradients.
FGMs can be also fabricated under a centrifugal force, by which it is possible to produce the FGMs with continuous gradients. Fabrication methods of FGMs under the centrifugal force are classified into three categories, as shown in Fig. 3, namely centrifugal method (application of centrifugal casting, and shown in Fig. 3 (a)), centrifugal slurry method (centrifugal sedimentation, and shown in Fig. 3 (b)) and centrifugal pressurization method (simple pressurization by the centrifugal force, and one example is shown in Fig. 3 (c)).
In case of centrifugal method shown in Fig. 3 (a), a centrifugal force applied to a homogeneous molten metal, dispersed with ceramics particles or intermetallic compound particles, drives the formation of the desired gradation. The composition gradient is then achieved primarily by the difference in the centrifugal force produced by the difference in density between the molten metal and solid particles(Fukui, 1991, Watanabe et al., 1998). It is known that the motion of particles in a viscous liquid under a centrifugal force obeys the Stokes' law(Kang&Rohatgi, 1996, Watanabe et al., 1998, Ogawa et al., 2006)
In contrast, slurry with two types of solid particles, high-velocity particle and low-velocity particle, is subjected to the centrifugal force during the fabrication of FGMs by the centrifugal slurry method(Watanabe et al., 2010), as shown in Fig. 3 (b). After complete sedimentation occurs, liquid part of the slurry will be removed, and therefore, it does not become a part of FGM.
Third one is the centrifugal pressurization method, by which the centrifugal force is only used for simple pressurization. In this method, compositional gradation should be formed prior the application of centrifugal force. Watanabe et al. are developing a centrifugal mixed-powder method, shown in Fig. 3 (c)(Watanabe et al., 2009), and a reactive centrifugal casting method(Watanabe et al., 2004a), which belong thiscategory. In this chapter, some results from the centrifugal method, centrifugal slurry method, centrifugal mixed-powder method and reactive centrifugal casting method will be described.
2. Centrifugal method
Centrifugal casting is a pressure casting, in which the force ofgravity is enhanced by spinning the mould. Generally, the segregation, caused by the density-difference betweenparticles and molten metal,must be avoided. However, it ispossible to create a compositional gradient due to the difference in materialdensity (Fukui, 1991, Watanabe et al., 1998).
Figure 4 shows the apparatus used for the centrifugal method. The ingot is melted and then theplug is pulled out to cast the molten metal directly into the spinning mould through the inlet. The spinning mould is preheated before the casting. The magnitude of the centrifugal force is expressed in
The composition gradient formed by the centrifugal method is affected by the difference in density between particles and a molten metal, the applied
2.1. Ceramic-particle dispersed FGMs fabricated by the centrifugalmethod
The typical microstructure of the Al/SiC FGM fabricated by the centrifugal methodis shown in Fig.5(Fukui & Watanabe,1996), wherethe applied
Figure 6 shows the histogram of the ceramic-particle volume fraction of the Al/SiC FGM fabricated by the centrifugal method (Fukui & Watanabe,1996). In this figure, the abscissa represents the position in the thickness direction of the ring, normalized by the thickness,
As described in introduction, the motion of ceramic particles in a viscous liquid under a centrifugal force can be estimated using Stokes' law. Therefore, in the FGMs fabricated by the centrifugal method, the mean particle size is distributed gradually along the applied centrifugal force. Figure 7 shows the particle distributions in the FGM fabricated by the centrifugal method (Watanabeet al., 2002). Note that the volume fraction of particles gradually increases towards the outer region. The most remarkable result shown in this figure is that the average particle size at the outer region is larger than that at the inner region, and the average particle size is gradually distributed in the FGMs. Although the data are not presented here, it has also been found that the particle size gradient in the FGM becomes steeper with increasing the
2.2Intermetallic-particle dispersed FGMs fabricated by the centrifugalmethod
Intermetallic compound particles could be also applicable for the centrifugal method as dispersed particles. The fabrication of the intermetallic compound particles dispersed FGMs by the centrifugal method can be classified into two categories based on the relation between the processing temperature and the liquidus temperature of master alloy(Watanabeet al., 2005). If the liquidus temperature of the master alloy is significantly higher than the processing temperature, as shown in Fig. 8 (a), the dispersed phase remains solid in a liquid matrix during the centrifugal casting. Alternatively, if the liquidus temperature of the master alloy is lower than the processing temperature,as shown in Fig. 8 (b), centrifugal force can be applied during the solidification both to the dispersed phase and to the matrix. These methodsare referred to as a centrifugal solid-particle method and a centrifugal
2.2.1. Centrifugal solid-particle method
Since the liquidus temperature of Al-5mass%Ti alloy, containing 11vol% Al3Ti platelets in the Al matrix, is about 1160°C and the processing temperature is 840°C of a liquid-solid coexisting temperature, the Al3Ti platelets remain solid in the liquid Al matrix and a centrifugal force is worked directly to platelets during the casting process.
Figure 9 shows typical microstructures of an Al/Al3Ti FGM fabricated under
It is known that volume fraction, size, shape and orientation of reinforcements in composite play an important role in improving the mechanical properties of the materials. Therefore, the Al/Al3Ti FGMs with oriented Al3Ti platelets should have an anisotropic wear resistance(Watanabeet al., 1999). The anisotropic wear resistances in the Al/Al3Ti FGMs were measured in three directions, namely along the longitudinal direction on outer surface of the ring (A), along the radial direction on the radial plane (B), and along the hoop direction on the radial plane (C), and results are shown in Fig. 10 (Watanabeet al., 2008). The result for a pure Al specimen made by the same process is also shown in the figure for comparison. The
wear volumes in the Al/Al3Ti FGM are much smaller than that of pure Al. Anisotropic wear resistance was found to be dependent on the direction of the test wear relative to the Al3Ti platelet orientation. Specimen tested along the Al3Ti platelets thickness direction shows the smallest wear resistance among the three orientations due to the ease with which the Al3Ti platelets broke. Although the data is not presented here, a greater anisotropy in wear resistance was found for specimens with larger orientation parameters(Watanabeet al.,2008).
The master alloy ingot used for the fabrication of the Al/Al3Ni FGMs contains 20mass%Ni. The liquidus temperature of Al-20mass%Ni is about 780°C, whereas the processing temperature is 900°C.Therefore, the centrifugal force is applied directly to a liquid phase. Figures 11 (a), (b) and (c) show typical microstructures of an Al/Al3Ni FGM taken at the inner, the interior, and the outer regions of the ring, respectively(Watanabeet al., 2004b). As can be seen, the Al3Ni primary crystals are distributed graded manner in the specimen. Moreover, there is remarkable position dependence in the particle size, namely the smaller particlesare found at the outer region of the ring, and
It is also found that as the
To discuss the formation mechanism of the graded composition during the centrifugal
The formation mechanismof the graded composition in the A–B alloy by the centrifugal in-site method could be summarizedas follows(Watanabe and Oike. 2005). First, due to the density difference, partial separation of Aand B elements in the liquid state occurs. Then, a chemical composition gradient is formed before thecrystallization of the primary crystal. The primary crystal in the matrix appears to dependon local chemical composition. The primary crystal migrates according to density difference,and a further compositional gradient isformed.
In the case of FGMs fabricated by the centrifugal
3.Centrifugal slurry method
Although the powder metallurgy has many advantages to fabricate the FGMs, it is difficult to produce the FGMs with continuous gradients. By combination of the powder metallurgy and a centrifugal slurry method, this shortcoming can be overcome. For the centrifugal slurry method, slurry with two types of solid particles will beused, namely high-velocity particle with larger density and/or larger particle size and low-velocity particle with smaller density and/or smaller particle size, judging by eq. (1). The particles gradients can be controlled by the difference of migration rate between the two kinds of particles. After complete sedimentation occurs, liquid part of the slurry will be removed, and a green-body with continuous gradient can be obtained. The green-body is, then, subjected to sintering by SPS or other sintering methods, and finally an FGM with continuous gradient can befabricated.
Figure 14 shows migration velocities of Ti and ZrO2 particles under the centrifugal force(Watanabe et al., 2010),where the densities of Ti particle and ZrO2 particle are 4.5Mg/m3 and 5.95Mg/m3, respectively. It is obvious that the velocity of ZrO2 particle is higher than that of Ti particle, when the particle size is same, due to its larger density. In this condition, Ti particle and ZrO2 particle become low-velocity particle and high-velocity particle, respectively. On the other hand, if the slurry contains the smaller ZrO2 particlesand larger Ti particles, the Ti particles can have high velocity in a specific condition.
Compositional gradient of the FGM fabricated by the centrifugal slurry method is calculated by simulation for the system with 90~150 µmparticle sized Ti and 38~75 µmparticle sized ZrO2 particle. In this case, Ti particle and ZrO2 particle becomes high-velocity particle and low-velocity particle, respectively. Results are shown in Fig. 15 (a) (Watanabe et al., 2010). Here, the horizontal axis is the normalized position of the green-body, and 0.0 and 1.0 correspond to the top and bottom surfaces of the settled green-body, respectively. It is clear from this figure thatcontinuous gradient can be obtained by the centrifugal slurry method. However, large compositional gradient, from 0 vol% at one end to 100 vol% at another end of the FGM for specific component, cannot be achieved. This is because the low-velocity particles (ZrO2 particle) placed at the bottom region before the sedimentation still may remain around same region after the complete sedimentation.
To overcome the above shortcoming, a slurry pouring method has been proposed to fabricate the FGM with large compositional gradient(Watanabe et al., 2010). First, solvent of the slurry is inserted into a spinning mould, as shown in Fig. 16 (a). Next, the slurry with two types of solid particles is poured into the spinning mould with solvent zone, as shown in Fig. 16 (b). Then, two types of solid particles migrate toward the centrifugal force direction, as shown in Fig. 16 (c). The existence of solvent zone increases the sedimentation period. As a result, large compositional gradient, for example from 0vol% at one end to 100vol% at another end, can be fabricated.
The computer simulation is conducted for the centrifugal slurry-pouring method, and results are shown in Fig. 15 (b), here thewidth of solvent zone is 100mm(Watanabe et al., 2010). It is clear from this figure that the FGM has a continuous gradient. It should be pointed out that the volume fraction of Ti at the normalized position of 0.0 is 0%, while 100% at 1.0 position. Thus, a large compositional gradient can be achieved by the centrifugal slurry-pouring method.
In order to verify and confirm the above simulation results, experiments were also conducted without and with the solvent zone. For simplicity, centrifugal force is not applied and particles were allowed to settle by gravity. After complete settlement of the particles, liquid is removed and the green-body is dried. The green-body was sintered by SPS method at 1300 °C for 5 minutes under applied stress of 30 MPa. FGMs obtained by SPS method have cylindrical shape with 20 mm in diameter.
Figures 17 (a) and (b) show experimental results of volume fractional gradients within the FGMs fabricated by the centrifugal slurry method (width of solvent zone is 0mm) and centrifugal slurry-pouring method (width of solvent zone: 100mm), respectively(Watanabe et al., 2010). Without the solvent zone, compositional gradient is limited as shown in Fig. 17 (a), whereas large compositional gradient, the range is between 0vol% and 100vol%, is achieved by the centrifugal slurry method with the solvent zone (the centrifugal slurry-pouring method). Good agreement is found between the experimental and calculated profile.
4. Centrifugal pressurization method
4.1. Centrifugal mixed-powder method
As a more developed fabrication method of FGMs under the centrifugal force, the centrifugal mixed-powder method was recently proposed by Watanabe et al.(Watanabe et al., 2009). As a first step of the process, a powder mixture of matrix metal particles,
Cu-30vol%SiC mixed-powder wasfabricated using pure Cu particles (99.9%, 1 mm and < 45μm in diameter) and SiCparticles (150 μm). Using thismixed-powder, Cu/SiC FGM was fabricated by the centrifugal mixed-powder method using vertical-type centrifugal casting machine. The applied centrifugal force was
When the Cu/SiCFGM was removed from the mould, no powders dropped out. Therefore, it is considered that all of the SiC particles in the powder mixture remained in the Cu/SiC FGM. SiC particles are observed on the outer surface of the specimen, as shown in Fig. 19 (a) (Watanabe et al., 2009). Moreover, the SiC particles are embedded in Cu matrix, as shown in Figs. 19 (b) and (c). It is found that SiC particles are successfully distributed on the surface of the FGMs by the centrifugal mixed-powder method, and the SiC particles are homogeneously distributed on the surface
4.2. Reactive centrifugal casting method
Matsuura et al. developed a new technique named reactive casting, which involves an exothermic reaction between elemental liquids, and enables one to produce the liquid of a high melting point intermetallic compound without the need for external heating(Matsuura et al., 2000). A combination of the reactive casting and centrifugal casting can be applied to the fabrication of a Ni-aluminide / steel clad pipe having an excellent resistance to corrosion and oxidation as well as a considerable level of toughness. This novel method is named as a reactive centrifugal casting method(Watanabe et al., 2004a, Watanabe et al., 2011). Ni powder was placed on a spinning steel pipe, as shown in Fig. 19 (a), and molten Al was poured into the steel pipe, as shown in Fig. 19 (b). The molten Al and Ni powder exothermically reacted and produced a composite layer consisting of Ni-aluminides on the inner surface of the steel pipe, as shown in Fig. 19 (c). The heat generated by the exothermic reaction melted the inner surface of the steel pipe and bonded the composite layer to the steel. Since inexperience Al ingots are used insteadof the experienced Al powder, this process will reduce the productioncost.
Figure 20 shows the SEM photograph of specimen fabricated under
Functionally graded materials (FGMs) can be fabricated under a centrifugal force, by which it is possible to produce the FGMs with continuous gradients. Fabrication methods of FGMs under the centrifugal force are classified into three categories, namely centrifugal method, centrifugal slurry method and centrifugal pressurization method. We have emphasized the use of the FGM fabrication methods under the centrifugal force as ones of the practical methods, since it has the feasibility of scaling up to mass production at a low cost. Although this chapter is mainly based on the studies by the authors, some other investigators have also fabricated FGMs using a similar method. The research activity in this field is continually increasing.
This work is supported by “Tokai Region Nanotechnology Manufacturing Cluster in KNOWLEDGE CLUSTER INITIATIVE” by the Ministry of Education, Culture, Sports, Science and Technology of Japan. One of the authors (YW) gratefully acknowledges the financial support from “The Light Metal Educational Foundation Inc. of Japan”.
Fukui Y. 1991 Fundamental Investigation of Functionally Gradient Material Manufacturing System using Centrifugal Force.
Fukui Y. Watanabe Y. 1996 Analysis of Thermal Residual Stress in a Thick-Walled Ring of Duralcan Base Al-SiC Functionally Graded Material,
( Hattori Y. Sato H. Miura-Fujiwara E. . Watanabe Y. 2010).Estimation of the Cooling Rate Distribution by means of Lamellar Spacing of Eutectic Structure during Fabrication of FGM under Centrifugal Force,
( Kang C. G. . Rohatgi P. K. 1996).Transient Thermal Analysis of Solidification in a Centrifugal Casting for Composite Materials Containing Particle Segregation.
( Matsuura K. Jinmon H. Hirashima Y. Khan T. I. Kudoh M. 2000).Reactive Casting of Ni-Al-Fe Ternary Intermetallic Alloys.
Miyamoto Y. Kaysser W. A. Rabin B. H. Kawasaki A. Ford R. G. . Edts. 1999 Functionally Graded Materials: Design, Processing and Applications,Kluwer Academic Publishers, 0-41260-760-3USA.
Ogawa T. Watanabe Y. Sato H. Kim-S I. Fukui Y. 2006 Theoretical Study on Fabrication of Functionally Graded Material with Density Gradient by a Centrifugal Solid-Particle Method,
( Sequeira P. D. Watanabe Y. Eryu H. Yamamoto T. Matsuura K. 2007).Effects of Platelet Size and Mean Volume Fraction on Platelet Orientation and Volume Fraction Distributions in Functionally Graded Material Fabricated by a Centrifugal Solid-Particle Method.
( Suresh S. Mortensen A. 1998). Fundamentals of Functionally Graded Materials, Processing and ThermomechanicalBehaviour of Graded Metals and Metal-Ceramic Composites,Communications Ltd., 1-86125-063-0UK.
- 10. Uemura, S.; Noda, Y.; Shinohara, Y. & Watanabe, Y. (ed.) (2010).Development and Technology of Functionally Graded Materials (in Japanese), CMC Publishing Co.,Ltd., ISBN 978-4-7813-0123-5, Tokyo, Japan.
( Watanabe Y. Yamanaka N. Fukui Y. 1998). Control of Composition Gradient in a MetalCeramic Functionally Graded Material Manufactured by the Centrifugal Method.
( Watanabe Y. Yamanaka N. Fukui Y. 1999). Wear Behavior of Composite Manufactured by Centrifugal Method. Metall. Mater. Trans. A, 30A 12(December, 1999), 3253 3261, 1073-5623
( Watanabe Y. Eryu H. Matsuura K. 2001).Evaluation of Three-Dimensional Orientation of Al3Ti Platelet in Al based FGMs Fabricated by aCentrifugal Casting Technique.
( Watanabe Y. Kawamoto A. Matsuda K. 2002).Particle Size Distributions of Functionally Graded Materials Fabricated by Centrifugal Solid-Particle Method.
( Watanabe Y. Watanabe S. Matsuura K. 2004a).Nickel-Aluminides/Steel Clad Pipe Fabricated by ReactiveCentrifugal Casting Method from Liquid Aluminumand Solid Nickel.Metall. Mater. Trans. A, 35A 5(May, 2004), 1517 1524, 1073-5623
( Watanabe Y. Sato R. Matsuda K. Fukui Y. 2004b).Evaluation of Particle Size and Particle Shape Distributions in 3FGMs Fabricated by a Centrifugal
( Watanabe Y. Kim-S I. Fukui Y. 2005).Microstructures of Functionally Graded Materials Fabricated by Centrifugal Solid-Particle and
Watanabe Y. Oike S. 2005Formation Mechanism of Graded Composition in Al-Al2Cu Functionally Graded Materials Fabricated by a Centrifugal insitu Method.
( Watanabe Y. Sato H. Fukui Y. 2008). Wear Properties of Intermetallic Compound Reinforced Functionally Graded Materials Fabricated by Centrifugal Solid-particle and In-Situ Methods.
Watanabe Y. Inaguma Y. Sato H. Miura-Fujiwara E. 2009 A Novel Fabrication Method for Functionally Graded Materials under Centrifugal Force: The Centrifugal Mixed-Powder Method.
( Watanabe Y. Miura-Fujiwara E. . Sato H. 2010).Fabrication of Functionally Graded Materials by Centrifugal Slurry-Pouring Method and Centrifugal Mixed-Powder Method.
( Watanabe Y. Inaguma Y. Sato H. 2011).Cold Model for Process of a Ni-aluminide/Steel Clad Pipeby a Reactive Centrifugal Casting Method.